Designation: B504 − 90 (Reappr (Reapproved oved 2011) 2011)
Endorsed by American Electroplaters’ Society Endorsed by National Association of Metal Finishers
Standard Test Method for
Measurement of Thickness of Metallic Coatings by the Coulometric Method1 This standard is issued under the ﬁxed designation B504; the number immediately following the designation indicates the year of original origin al adoption or, in the case of revis revision, ion, the year of last revision. revision. A number in paren parenthese thesess indicates the year of last reappr reapproval. oval. A superscript epsilon (´) indicates an editorial change since the last revision or reapproval. This standard has been approved for use by agencies of the Department of Defense.
area, the electrochemical equivalent of the coating metal, the anodicano dic-cur curren rentt ef effficie iciency ncy,, and the den density sity of the coa coatin ting. g. Alternatively, the equipment may be calibrated against standards with known coating thicknesses.
1. Sco Scope pe 1.1 This test method covers covers the determ determination ination of the thicknesss of meta nes metallic llic coatings coatings by the cou coulom lometr etric ic met method hod,, also known kno wn as the ano anodic dic sol solutio ution n or elec electro troche chemic mical al str stripp ipping ing method.
3.4 Commer Commercial cial instruments instruments using this princ principle iple are available. The method is rapid and versatile, but destructive to the coating. In general, its range is considered to be between 0.75 and 50 µm. Chromium, gold, tin, and other coatings can be measured down to 0.075 µm.
1.2 This standar standard d doe doess not purport purport to add addre ress ss all of the safet sa fetyy co conc ncer erns ns,, if an anyy, as asso socia ciated ted wi with th it itss us use. e. It is th thee responsibility of the user of this standard to establish appro priate safety and health practices and determine the applicability of regulatory limitations prior to use.
4. Signi Signiﬁcan ﬁcance ce and Use
2. Referenc Referenced ed Documents Documents
4.1 Measur Measurement ement of the thickness thickness of a coating is essential to assessing its utility and cost.
2.1 ISO Standard: ISO IS O 21 2177 77 Metal Metallic lic Coatin Coatings—M gs—Measur easurement ement of Coatin Coating g Thickness—Coulometric Method by Anodic Dissolution 2
4.2 The cou coulom lometri etricc meth method od des destro troys ys the coa coatin ting g ove overr a very small (about 0.1 cm 2) test area. Therefore its use is limited to applications where a bare spot at the test area is acceptable or the test piece may be destroyed.
3. Summ Summary ary of Test Test Method 3.1 The thickness thickness of the coating is determined by measuring measuring the quantity of electricity (coulombs) required to dissolve the coating anodically from a known and accurately deﬁned area.
5. Fact Factors ors Affect Affecting ing the Accuracy Accuracy of the Method 5.1 Composition of Electrolytes— Electrolytes Electrolytes used for coulometric lometr ic thi thickn ckness ess meas measure uremen ments ts mus mustt per permit mit the coa coating ting metal to dissol dissolve ve at a consta constant nt anodic anodic-curr -current ent ef effficiency (preferab er ably ly 10 100 0 %) %);; th they ey mu must st ha have ve a ne negl glig igib ible le sp spon ontan taneo eous us chemical effect on the coating metal and must so differentiate electrochemically between the coating and the substrate that a suitably sharp and large voltage change occurs at the end point of the test. 5.1.1 Electrolytes Electrolytes furni furnished shed with commer commercial cial instru instruments ments may be presumed to meet these requirements; others must be eval ev alua uated ted be befo fore re us usee by tes testin ting g st stan anda dard rdss ha havi ving ng kn know own n thicknesses. Appendix thicknesses. Appendix X1 lists some electrolytes and coatingsubstrate combinations that have been used with some instruments.
3.2 As com common monly ly pra practic cticed, ed, the meth method od emp employ loyss a sma small ll metal cell which is ﬁlled with an appropriate electrolyte. The test specimen serves as the bottom of the cell and an insulating gasket between the cell and the specimen deﬁnes the test area (about 0.1 cm 2). With the test specimen as anode and the cell as cathode, a constant direct current is passed through the cell until the coating has dissolved, at which time a sudden change in voltage occurs. 3.3 The thickness thickness of the coating may be calculated from the quantity quanti ty of electric electricity ity used (curr (current ent multiplied by time), the 1
This test method is under the jurisdiction of ASTM Committee B08 Committee B08 on on Metallic and Inorganic Coatingsand is the direct responsibility of Subcommittee B08.10 Subcommittee B08.10 on on Test Methods. Current Curre nt editio edition n approv approved ed Oct. 1, 2011 2011.. Publi Published shed October 2011. Origin Originally ally approved in 1970. Last previous edition approved in 2007 as B504 – 90 (2007). DOI: 10.1520/B0504-90R11. 2 Available from American National Standards Institute (ANSI), 25 W. 43rd St., 4th Floor, New York, NY 10036, http://www.ansi.org.
5.2 Current For cou coulom lometr etric ic ins instru trumen ments ts emCurrent Variation— For ploying the constant-current technique, variation of the current during dur ing a tes testt will result result in err errors ors.. For instrume instruments nts using a current-time integrator, variation of the current during a test will not result in error unless the current change is such as to
Copyright © ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959. United States
B504 − 90 (2011) displace the anodic current density beyond the range of constant or 100 % anodic-current efficiency.
used, the manufacturer’s instructions shall be followed insofar as they are compatible with this test method.
5.3 Area Variation— The accuracy of the thickness measurement will not be better than the accuracy with which the test area is deﬁned or known. Typically, this test area is deﬁned by a ﬂexible, insulating gasket. Area variation is usually minimized by using as large an area as practical and by using a constant pressure device. If excessive pressure is applied to such a gasket, the test area may be altered undesirably.
6.2 Calibration of Direct-Reading Instruments— Directreading instruments shall be calibrated against standards having known coating thicknesses, and adjusted to produce correct readings corresponding to the coating thicknesses of the standard. 6.3 Calibration of Nondirect-Reading Instruments: 6.3.1 Nondirect-reading instruments shall be calibrated against standards having a known coating thickness by using a calibration constant, C , calculated as follows:
5.4 Agitation— In most, but not all, coulometric thickness measurements, a relatively high anodic-current density is employed to shorten the test time. It is then necessary to agitate the electrolyte to maintain a constant anodic-current efficiency. Where agitation is required, insufficient agitation may result in polarization of the specimen, thereby causing a premature and false endpoint.
C 5 coating thickness of the standards/instrument reading
6.3.2 The instrument shall be adjusted so that where standards having known coating thicknesses are tested, the correct thickness is obtained by multiplying the instrument reading by the calibration constant, C .
5.5 Alloying Between Coatings and Metallic Substrates— The measurement of a coating thickness by the coulometric method implicitly assumes that a sharply deﬁned interface exists between the coating and the substrate. If an alloy layer exists between the coating and the substrate as, for example, in the case of coatings applied by hot dipping, the coulometric end-point may occur at some point within the alloy layer, thus giving a high value of the thickness of the unalloyed coating.
6.4 Thickness Standards— The thickness standards shall consist of the same type of coating and substrate as the specimens to be measured, and they shall have an accuracy of 65 % or better. 7. Procedure for Making Measurements 7.1 If commercial equipment is used, the manufacturer’s instructions shall be followed insofar as they are compatible with this test method.
5.6 Purity of Coating— Impurities or additives that codeposit with the coating may change the effective electrochemical equivalent of the coating and also change the anodic current efficiency. 5.6.1 Alloy Coating— Variations in the composition of alloy coatings will change the effective electrochemical equivalent of the coating.
7.2 The test surface shall be cleaned of all foreign material that might affect the measurement. NOTE 1—Certain nickel deposits, frequently dull nickel, may exhibit passivity. When such coatings are tested coulometrically, the voltage across the specimen and test cell is markedly higher (approximately 1 V) than normal, and the coating does not dissolve. Oxygen is evolved at the specimen and the test may continue indeﬁnitely. NOTE 2—Removal of the passivity may be accomplished in some cases by mildly abrading (as with a pencil eraser) the nickel surface prior to testing. Alternatively, the specimen may be made cathodic in the coulometric electrolyte for 10 to 20 s by applying current from an external source. Allowing the nickel to be in contact with 10 % volume hydrochloric acid for approximately 1 min prior to the test may also be used effectively.
5.7 Cleanliness of Test Surface— The surface to be tested must be clean. Oil, grease, and organic coatings such as lacquer must be removed with suitable solvents. Oxides, conversion coatings, and corrosion products are preferably removed by carefully burnishing the test surface with a clean, soft pencil eraser. Tin and nickel surfaces, in particular, should be so burnished prior to testing to remove passive oxide ﬁlms. 5.8 Density of Coating— The coulometric method intrinsically measures coating mass per unit area, the equivalent linear thickness being a function of the density of the coating. If the density of the coating tested is different from the value of the density used for the calibration, the linear thickness obtained coulometrically will be different from the actual linear thickness of the coating tested. 5.8.1 Density of Alloy Coatings— Variation in the composition of alloy coatings will change the density of the coating.
7.3 After completion of the measurement, the test surface shall be examined visually, and if the dissolution of the coating is not virtually complete, the measurement shall be discarded and repeated.
5.9 Number and Location of Tests— Since the coulometric test method measures, essentially, a local coating thickness, a single test may not be representative of the coating thickness over the entire signiﬁcant surface.
8.2 Instruments suitable for compliance with 8.1 are available commercially. For many coating systems the instruments are capable of making measurements with an uncertainty of less than 4 % (95 % conﬁdence).
8. Precision and Bias 8.1 The equipment, its calibration, and its operation shall be such that the coating thickness can be determined with an uncertainty of less than 10 %.
8.3 Although an uncertainty of less than 10 % may be achieved consistantly for a great number of coating-substrate combinations, the uncertainty may be greater when the coating thickness is less than 1µ m or exceeds 50 µm.
6. Calibration of Equipment 6.1 The equipment shall be calibrated by means of standards having known coating thicknesses. If commercial equipment is 2
B504 − 90 (2011) 8.4 The bias of a coulometric measurement is the discrepency remaining between the measured thickness and the true thickness if all random errors are eliminated. It is, therefore, no
greater than, and attributable to (1), the calibration error of the instrument and (2) the quality of the calibration standard used to calibrate the instrument.
APPENDIX (Nonmandatory Information) X1. ELECTROLYTES TABLE X1.1 Typical Electrolytes for Electrodeposited Coatings A
X1.1 Table X1.1 lists electrolytes that have been used for coulometric thickness measurements; however, they are not necessarily suitable for use with all types of coulometric instruments.
Substrate (Basis Metal) Coating
Cadmium Chromium Copper Lead Nickel Silver Tin Zinc
X1.2 Use of these electrolytes is not mandatory for compliance with this method, and when commercial coulometric instruments are used, the manufacturer’s recommendations shall be followed. X1.3 Table X1.2 lists other coating-substrate combinations that have been used successfully with commercially available electrolytes.
Steel 1, 10 2, 11 5, 14 17 6, 18 7 3, 4, 20 9
Copper and Alloys (such as brass) 1, 10 3, 4, 12 ... 17 6, 19 8 3, 4, 20 9
Nickel 1 2, 13 5, 15 17 ... 7 3, 4 9
Aluminum Zinc 1 2, 13 5 ... 6, 18 ... 2, 21 9
... ... 16 ... ... ... ... ...
The numbers in the table refer to the following aqueous solutions: (1) 100 g KI/L, with traces of I2 (2 ) 100 g Na2SO4 /L (3 ) 175 mL HCl (sp gr 1.18)/L (4 ) 150 g NaOH/L (5 ) 80 g NaKC4H4O6 (sodium potassium tartrate) + 100 g NH4NO3 /L (6 ) 30 g NH4NO3 + 30 g NaSCN/L (7 ) 100 g NaNO3 + 3 ml HNO3 (sp gr 1.42)/L (8 ) 180 g KSCN/L (9 ) 100 g NaCl or KCl/L (10 ) 30 g KCl + 30 g NH4Cl/L (11) 100 mL H3PO4 (sp gr 1.75) + 10 g CrO 3 /L (12 ) 100 g Na2CO3 [for coatings up to 5 µm (0.2 mil)]/L (13 ) 64 mL H3PO4 (sp gr 1.75)/L (14 ) 800 g NH4NO3 + 10 mL NH4OH (sp gr 0.88)/L (15 ) 100 g K2SO4 + 20 mL H3PO4 (sp gr 1.75)/L (16 ) Pure H2SiF6 solution containing notless than 30 % H2SiF6 (Slightly weaker acid may be used, if some MgSiF6 is added to the solution.) (17 ) 200 g CH3COONa + 200 g CH3COONH4 /L (18 ) 800 g NH4NO3 + 3.8 g CS(NH2)2 (thiourea)/L (19 ) 100 mL HCl (sp gr 1.18)/L (20 ) 100 g KNO3 + 100 g KCl/L (21) 50 mL H2SO4 (sp gr 1.84) + 5 g KF/L
B504 − 90 (2011) TABLE X1.2 Measurable Coating-Substrate Combinations Substrate Coating
BrassA Cobalt Gold Indium Iron Nickel (Electrodes)A Nickel-IronA Tin-LeadA Tin-NickelA Tin-ZincA
Copper and Copper Alloys
X X X X
X X X X X X
X X X X
Magnetic Stainless Steel
X X X
The measurement accuracy of these alloy coatings is dependent on the composition of the coating.
ASTM International takes no position respecting the validity of any patent rights asserted in connection with any item mentioned in this standard. Users of this standard are expressly advised that determination of the validity of any such patent rights, and the risk of infringement of such rights, are entirely their own responsibility. This standard is subject to revision at any time by the responsible technical committee and must be reviewed every ﬁve years and if not revised, either reapproved or withdrawn. Your comments are invited either for revision of this standard or for additional standards and should be addressed to ASTM International Headquarters. Your comments will receive careful consideration at a meeting of the responsible technical committee, which you may attend. If you feel that your comments have not received a fair hearing you should make your views known to the ASTM Committee on Standards, at the address shown below. This standard is copyrighted by ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States. Individual reprints (single or multiple copies) of this standard may be obtained by contacting ASTM at the above address or at 610-832-9585 (phone), 610-832-9555 (fax), or [email protected]
(e-mail); or through the ASTM website (www.astm.org). Permission rights to photocopy the standard may also be secured from the ASTM website (www.astm.org/ COPYRIGHT/).